86 4.2 Recombination Dynamics

initial enhanced trap repair

ωem

|a〉

|b〉

|a〉

|b〉

Figure 4.7: Scheme of Nanoplatelet Subensembles. Illustration of the whole NPl ensemble before and after the postsynthetic trap repair process. Two subensembles are involved in this picture: defect-containing dark NPls with a strong tendency towards nonradiative recombination and defect-free bright NPls which predominantly undergo radiative recombination.

For the purpose of validating this theoretical model, transient absorption spectroscopy (TAS) was
employed. As shown inEquation 3.4andEquation 3.5, the measured data obtained with the help
of this time-resolved technique may either be presented asΔ𝑂𝐷(𝜆)or asΔ𝑇 (𝜆)/𝑇_{0}(𝜆), respectively.

Therefore, as mentioned inSubsection 3.3.2, the measurement technique may also be referred to as differential transmission spectroscopy (DTS) instead of TAS.

### a

ODΔT/T0ΔT/T0

400 450 500

wavelength in nm 0.2

0.3

0.1 0.10

0

1 ps

3000 ps

pulse delay time in ps500 1500

0 1000

0.1 0.08 0.06 0.080.1 0.06 0.04

enhanced initial

3 ML EC

E1s

### b

### c d

ΔT/T0

Figure 4.8: Differential Transmission Spectroscopy on CsPbBr_{3} Nanoplatelets. (a)Steady-state
absorption spectrum of a 3 ML CsPbBr_{3}NPl dispersion.(b)Differential transmission spectra of the same
sample at delay times ranging from 1–3000 ps.(c)Transient of the differential transmission at the energetic
position of the exciton𝐸_{1s}, as shown in (a), for a dispersion that has not been treated with the enhancement
step.(d)The respective DTS transient for a NPl dispersion that underwent the trap repair process.

Figure 4.8 ashows the steady-state absorption spectrum of the dispersion containing 3 ML NPls. As discussed before forFigure 4.4 b, the absorption spectra before and after the trap repair are basically identical. For the examination of the time-resolved absorption, a pump pulse excitation wavelength of 400 nm (≈3.1 eV) was applied. The corresponding DTS spectra for the nonenhanced dispersion are

88 4.2 Recombination Dynamics
plotted inFigure 4.8 b. The dominant bleaching peak at around 452 nm within these spectra reveals
that already 1 ps after excitation the main population of excited e-h pairs is energetically located at
the exciton peak (arrow𝐸_{1s}inFigure 4.8 a). This shows that excitons predominantly determine the
behavior of these strongly confined NPls, since the bleaching peak appears well below the continuum
onset𝐸_{C}.^{199}

To study exciton recombination dynamics, we observe two DTS transients at the position of this
population𝐸_{1s}: one before enhancement (initial) shown inFigure 4.8 cand one after enhancement
(enhanced) plotted inFigure 4.8 d. The NPls in dispersion are spaced far apart with respect to each
other and are hence considered to be independent, i.e., there is no charge or energy transfer between
them. If one of these independent NPls is photoexcited, it may contain one or even several e-h pairs
(cf.Subsection 2.3.3). A fast initial signal drop may be observed for both curves inFigure 4.8 c and
d, also highlighted by a steep dashed grey line. This process relates to nonradiative exciton-exciton
annihilation, dominantly occurring when a NPl initially contains more than one exciton. Its magnitude
is strongly dependent on the excitation density and it dominates the temporal evolution of the exciton
decay until only one exciton per photoexcited NPl remains.^{200}This will be discussed in greater detail
within the next subsection.

Another dashed line in both plots indicates that the remaining decay (𝑡_{delay}>100 ps) may be described
by a single monoexponential function for the enhanced NPl dispersion inFigure 4.8 d, whereas this is
not possible for the initial sample represented inFigure 4.8 c. The model proposed above inFigure 4.7
considers an overall ensemble of NPls consisting of two subensembles. Consequently, the transients in
Figure 4.8 c and dshould be a superposition of the DTS signals stemming from the two subensembles.

On the long time scale for𝑡_{delay}>100 ps, the measured curve for the initial sample actually requires
the sum of two exponential functions for a proper representation, indicating a well-balanced presence
of both subensembles. However, the curve for the enhanced sample may be described by a single
exponential function within the same time range. This behavior is typical for excitonic recombination
and indicates that the overall sample consists predominantly of the subensemble representing NPls
which are considered to be defect-free after the repair process. All in all, this observation is further
proof for the efficiency of the trap repair process within the NPls.^{20}

A similar behavior may also be observed in time-resolved PL spectra obtained with TCSPC.Figure 4.9 shows the respective data before and after enhancement for all NPl dispersions and also for two films comprising 3 ML NPls. Compared to TAS, TCSPC offers the opportunity to access longer delay times with the drawback of a worse temporal resolution (cf. Section 3.3). Therefore, fast processes like exciton-exciton annihilation cannot be determined accurately as they are superimposed and smeared out by the broader instrument response function. Hence, this data should be interpreted with caution, especially for very short time delays.

Similar to the results presented above, the enhanced samples (blue curves) shown inFigure 4.9may be described by a monoexponential function, delivering further proof that only the subensemble with repaired NPls plays a role after the enhancement. On a short timescale, lifetimes seem to extend when repairing the NPl surface. Only when the population already dropped to a few percent, it seems as if some trap states might cause long-lived excitons in the initial samples (this can be observed best for the black curves inFigure 4.9 b and d). Interestingly, the graphs inFigure 4.9 cshow the general trend for NPl films to show faster decay rates as compared to the NPls in dispersion which are represented in the other panels. This trend is rooted in the possibility of interaction between the NPls in films

### a

2 ML

### b

5 ML

### c

3 ML

### f

6 ML

### d

4 ML

### e

time in ns 0.1

0.01 1

PL intensity in a.u.

10 20 30 40

0 time in ns

0.1

0.01 1

PL intensity in a.u.

10 20 30 40

0

time in ns 0.1

0.01 1

PL intensity in a.u.

10 20 30 40

0 time in ns

0.1

0.01 1

PL intensity in a.u.

10 20 30 40

0

time in ns 0.1

0.01 1

PL intensity in a.u.

10 20 30 40

0 time in ns

0.1

0.01 1

PL intensity in a.u.

10 20 30 40

0 3 ML

Figure 4.9: Time-Resolved PL of CsPbBr3Nanoplatelets. (a),(b),(d),(e), and(f)PL decay curves of initial (black lines) and enhanced (blue lines) NPl dispersions of 2–6 ML NPls, respectively. (c)The corresponding curves for films of the 3 ML sample. The insets present photos of initial (left) and enhanced (right) NPl samples under UV-light illumination.

and shows that the assumption of independent individual NPls — as introduced for dispersions — is not valid in this case. Moreover, it is always important to keep in mind that time-resolved TAS and PL do not necessarily exhibit the same decay curves. TAS represents the sum of electron and hole populations, whereas TCSPC is a representative of the product of these populations.

90 4.2 Recombination Dynamics 4.2.2 Exciton-Exciton Annihilation

Next, the influence of the NPl thickness on exciton-exciton annihilation shall be studied. Figure 4.8 c
and dalready gave an impression on how this effect has an impact on the decay curves recorded with
DTS. In the following, this fast process will be studied for the nonenhanced NPls only. The lifetime
𝜏_{2}shall be extracted for dispersions of such samples (cf.Figure 2.11andEquation 4.2). Exemplarily,
the DTS data is illustrated for the 2 ML dispersion inFigure 4.10 afor which different pump pulse
energies, i.e., different excitation densities, were employed. The respective decay curves of the exciton
population exhibit a fast decay component within the first tens of picoseconds, the amplitude of which
shows a strong correlation to the excitation density. This strong dependence and the total absence of
this effect at very low excitation densities are clear indications for a multi-exciton process, namely
exciton-exciton annihilation.

### a

excitation density in 100.8 ^{-4} J/cm^{2}

0 1.2

### b

1.6 0.4

0 1 2 3 4 5

0 0

0.02 0.04 0.06 ΔT/T0

1 0.5 80

0 20 40 60 100 120

pulse delay time in ps 0

ΔT/T0

2

1

2 ML

1.5·10^{-4} J/cm^{2}
6.0·10^{-6} J/cm^{2}

〈N〉

〈N〉, N≥1)P(

Figure 4.10: Excitation-Density Dependence of the Exciton Decay in Nanoplatelets. (a)Exciton
population decay at the bleaching peak for 2 ML NPls at different excitation densities. Inset left: After the
fast decay via exciton-exciton annihilation an initially excited NPl contains at most one exciton. Inset
right: Above a certain excitation density the DTS signal saturates, meaning that almost every NPl was
initially excited with at least one exciton.(b)Saturation behavior of the DTS curves from (a) averaged over
longer pulse delay times 1 ns≤ 𝑡_{delay}≤3 ns. The blue curve is fitted in accordance with Poisson statistics
and allows for the determination of the exact proportionality between the excitation density𝐽_{ex}and the
initial average number of excitons per NPl after excitation⟨𝑁 ⟩. The shaded grey area highlights the range
0.3 < ⟨𝑁 ⟩ < 0.4chosen to analyze the exciton-exciton annihilation lifetime𝜏_{2}.

As indicated in the left inset of this figure, this effect subsides after some tens of picoseconds. It
may be assumed that by far the largest proportion of all initially excited NPls contains only one
remaining exciton at most at this point in time which already has been introduced inFigure 2.12and
is referred to as𝑡_{1}in this model. For the measurement presented inFigure 4.10 aa value of around
100 ps is determined for𝑡_{1}. After this time, in the confines of this assumption, only monomolecular
recombination of single excitons — via radiative or non-radiative channels — is possible.

Since the rates for exciton-exciton annihilation and for monomolecular recombination differ strongly (cf. Figure 2.11), the following assumption may be made and based thereon a simpler function is derived from Poisson statistics.

𝑃 (⟨𝑁 ⟩, 𝑁 = 1, 𝑡 = 𝑡_{1}) ≈ 𝑃 (⟨𝑁 ⟩, 𝑁 ≥ 1, 𝑡 = 0)

= 1 − 𝑃 (⟨𝑁 ⟩, 𝑁 = 0, 𝑡 = 0)

= 1 −⟨𝑁 ⟩^{0}
0! 𝑒^{−⟨𝑁 ⟩}

= 1 − 𝑒^{−⟨𝑁 ⟩}

(4.3)

Therefore, the fraction of NPls containing exactly one exciton at time𝑡_{1}may be estimated via a function
𝑓 (⟨𝑁 ⟩) = 1 − 𝑒^{−⟨𝑁 ⟩}only dependent on⟨𝑁 ⟩as demonstrated inEquation 4.3.

As mentioned above, exciton-exciton annihilation processes can effectively be assumed to be over
at around𝑡_{1}. Accordingly, the overall decay behavior, i.e., the shape of the decay curve, should be
excitation density independent after this point in time. The excitation density only determines how
many NPls are excited with at least one exciton at𝑡 = 0or, put in other words, how many NPls are
excited with exactly one exciton at𝑡 = 𝑡_{1}(cf.Equation 4.3). Naturally, there is a maximum amount
of NPls that can be excited and this is the total number of observed NPls𝑛_{total} as introduced in
Subsection 2.3.3. Therefore, theΔ𝑇 /𝑇_{0}intensity at𝑡 = 𝑡_{1}is expected to converge against a saturation
limit with increasing excitation density 𝐽_{ex}. This limit represents the case that each of the 𝑛_{total}
observed NPls contains exactly one remaining exciton at𝑡 = 𝑡_{1}. This saturation behavior is actually
shown in the right inset inFigure 4.10 a. Since the decay curves follow the same trend, the values of
the transients may be averaged and plotted versus the excitation density as shown inFigure 4.10 b. As
indicated by the solid blue curve, these data points may be fitted by a function𝑔 (𝐽_{ex}) = 𝑎 (1 − 𝑒^{−𝑏⋅𝐽}^{ex}).

The fitting parameters𝑎 and 𝑏may be used to add a new pair of axes on the top and the right

ΔT/T0 in a.u.

0.4 1

0.6 0.8

pulse delay time in ps

10 40

0 20

2 ML

3 ML

4 ML

5 ML 6 ML

30

Figure 4.11: Exciton-Exciton Annihilation Lifetime Analysis for All Nanoplatelets. DTS decay curves at the excitonic peak for all samples 2–6 ML with an excitation density corresponding to0.3 < ⟨𝑁 ⟩ <

0.4(marked by dots). Solid lines represent exponential fit functions. For better comparison the graphs have been normalized with respect to these fit functions.

92 4.2 Recombination Dynamics
side of Figure 4.10 b. In relation to these axes the fitted blue curve then represents the function
𝑓 (⟨𝑁 ⟩) = 1 − 𝑒^{−⟨𝑁 ⟩}as given inEquation 4.3. Consequently, the proportionality factor between⟨𝑁 ⟩
and𝐽_{ex}is determined and the fraction of initially optically excited NPls𝑃(𝑁 ≥ 1)may be extracted
from the plot either versus𝐽_{ex}or⟨𝑁 ⟩. InSubsection 2.3.3we stated that⟨𝑁 ⟩should be in the range of
0.3 − 0.4in order to determine𝜏_{2}. This range is shaded in light grey withinFigure 4.10 band thereby it
is revealed that exactly one of the initial DTS measurements fulfills this requirement. This procedure
was repeated for all NPl samples. The corresponding initial decay curves attributed to exciton-exciton
annihilation are plotted inFigure 4.11where the condition0.3 < ⟨𝑁 ⟩ < 0.4holds true for all data.

A clear trend is observable in this graph. The decay becomes faster for thinner NPls which is even
easier to observe in the highlighted exponential fits. The lifetimes𝜏_{2}can be extracted therefrom and
are presented inTable 4.1.

Table 4.1: Exciton-Exciton Annihilation Lifetimes.The exciton-exciton annihilation lifetimes𝜏2are extracted fromFigure 4.11for all NPl samples.

2 ML 3 ML 4 ML 5 ML 6 ML

𝜏_{2}in ps 6.9 ± 0.2 8.0 ± 0.2 13.3 ± 0.2 29.1 ± 0.7 65.9 ± 1.4

The so-called “universal volume scaling law”^{123}suggests a linear dependence between the lifetime𝜏_{2}
and the volume of small NCs.^{201}Therein,𝜏_{2} also denotes the lifetime via which the amount of e-h
pairs in a NC is reduced from two to one. Due to their small size such NCs are also often referred to
as quantum dots (QDs), even for the case of weak confinement only. Mostly, this law is confirmed
for the case of spherical or cubic NCs.^{202}However, the trend observed in our case does not reflect
this dependence. For the CsPbBr_{3} NPls presented here, the volume is directly proportional to the
thickness since the lateral size is not changed. Clearly, there is no linear dependence between𝜏_{2}
and NPl thickness inTable 4.1which suggests that the “universal volume scaling law” should not be
applied to strongly confined LHP NPls.

It has also been suggested that the “universal volume scaling law” is not valid for CdSe NPls.^{203}
Li et al. derived that the size tuning of a weakly confined lateral dimension mainly influences the
collision frequency of excitons, whereas the size tuning of the strongly quantum confined thickness
mostly influences the interaction probability during a collision. They extracted a dependence of the
exciton-exciton annihilation lifetime𝜏_{2}on the NPl thickness which scales to the power of seven. The
data presented inTable 4.1for CsPbBr_{3}NPls exhibit a respective dependence to the power of five.

Generally, the𝜏_{2}values for CsPbBr_{3}NPls are short and amount to less than 70 ps even for the thickest
NPls. The lifetimes are similar to the values reported for spherical CdSe QDs^{123}and even faster than
the ones reported for CdSe NPls.^{203}

Lateral size-tuning of NPls would be beneficial to learn more about the exact influence of the NPl
geometry on the lifetime𝜏_{2}. However, this is unfortunately outside the scope of this study. Nevertheless,
even without this additional information, the trend presented inTable 4.1suggests a strong deviation
from the “universal volume scaling law” for perovskite NPls. Combining these results on CsPbBr_{3}NPls
with the ones of Li et al. on CdSe NPls leads to the assumption that the law might only be applicable
to spherical or cubic NCs, where all dimensions exhibit a similar degree of quantum confinement.

4.2.3 Monomolecular Recombination

In the previous subsection the exciton-exciton annihilation lifetime was deduced to lie in the range of tens of picoseconds. In contrast, lifetimes for monomolecular recombination within LHP NCs usually lie in the nanosecond range. Due to this significant difference of around two orders of magnitude it may safely be assumed that the two processes happen subsequently as already illustrated in the scheme ofFigure 2.12. In this subsection the exciton recombination dynamics following the exciton-exciton annihilation process will be studied for nonenhanced NPls in dispersions.

ΔT/T0 in a.u.

0 12

4 8

pulse delay time in ps

1000 3000

0 2000

2 ML

1.5·10^{-4} J/cm^{2}
6.0·10^{-6} J/cm^{2}

Figure 4.12: Differential Transmission Spectroscopy on 2 ML Nanoplatelets.DTS decay curves at
the excitonic peak for the 2 ML sample without postsynthetic trap repair. Different excitation densities
were applied (6.0⋅10^{−6}–1.5⋅10^{−4}J/cm^{2}) and all curves have been normalized to unity at𝑡_{delay}=1000 ps.

Illustrating the data this way clearly shows that all curves exhibit the same shape and decay for pulse delay times longer than a few hundreds of picoseconds. This means that monomolecular exciton recombina-tion within the NPl ensemble is an excitarecombina-tion density-independent process, contrary to exciton-exciton annihilation. The inset depicts the process of monomolecular recombination schematically, helping to understand this relation. Higher excitation densities only lead to a larger number of involved NPls, but the decay within each individual independent NPl — and therefore, also the decay behavior of the whole NPl ensemble — is not influenced.

Figure 4.12shows DTS transients at the 1s exciton position that are based on the same measurement
series asFigure 4.10 a. However, since the slower process of monomolecular recombination shall be
studied, a larger time delay range up to 3000 ps is presented here. The curves for different excitation
densities are normalized at𝑡_{delay}=1000 ps revealing that all graphs exhibit the same decay behavior
for longer delay times𝑡_{delay}≥200 ps. This proves that the monomolecular exciton population decay
behavior of the ensemble is not influenced by the excitation density.

Long-term recombination is investigated for all different NPl thicknesses inFigure 4.13. Since the
preceding exciton annihilation processes are of no importance for this investigation, the graphs are
only plotted for𝑡_{delay} ≥ 200 ps. As shown above, the excitation density𝐽_{ex} does not influence the
decay behavior, however, larger𝐽_{ex} lead to an enhanced SNR of the DTS signal. Therefore, values
𝐽_{ex} ≥0.5⋅10^{−4}J/cm^{2}were chosen for all samples. Looking at the plots withinFigure 4.13carefully,
one recognizes that the decay curves are not entirely monoexponential. A slight deviation from the
exact monoexponential decay occurs since nonenhanced NPls are examined in this case, therefore,
leaving the potential for the presence of two subensembles (seeFigure 4.7).

94 4.2 Recombination Dynamics

ΔT/T0 in a.u.

0.4 1

0.6 0.8

pulse delay time in ps

1000 3000

0 2000

2 ML 3 ML 4 ML 5 ML 6 ML

Figure 4.13: Recombination Lifetime Analysis for all Nanoplatelets.DTS decay curves for all NPl
samples at the respective 1s excitonic peak. In order to focus on the monomolecular exciton recombination,
all graphs are plotted for𝑡_{delay}≥200 ps only. The decay curves are normalized at𝑡_{delay}=500 ps and a clear
trend towards shorter recombination lifetimes𝜏_{1}may be observed for thinner NPls.

Nevertheless, the quantity to be extracted fromFigure 4.13for all NPl thicknesses is the monomolecular exciton recombination lifetime

𝜏_{1}= ( 1
𝜏_{1,r} + 1

𝜏_{1,nr})

−1

. (4.4)

Here, in this approximation𝜏_{1}simply represents a lifetime for each NPl ensemble without going further
into detail on the role of the subensembles. As illustrated in the inset ofFigure 4.12,Equation 4.4
takes into account all processes in which an exciton decays radiatively (𝜏_{1,r}) or nonradiatively (𝜏_{1,nr})
without interacting with another exciton. The lifetime𝜏_{1}should not be confused with the population
lifetime𝑇_{1}of the exciton ensemble as it has been introduced inSection 2.4.Equation 4.2shows that
the approximation𝑇_{1} ≈ 𝜏_{1}may only be made in the absence of exciton-exciton annihilation.

The lifetime values𝜏_{1}were extracted in the pulse delay time region 1500 ps≤ 𝑡_{delay}≤3000 ps for all
graphs ofFigure 4.13. The results are presented inTable 4.2.

Table 4.2: Monomolecular Recombination Lifetimes.The Monomolecular Recombination Lifetimes
𝜏_{1}are extracted fromFigure 4.13for all NPl samples.

2 ML 3 ML 4 ML 5 ML 6 ML

𝜏_{1}in ns 2.45 ± 0.08 2.95 ± 0.09 3.92 ± 0.19 6.05 ± 0.17 6.69 ± 0.14

The values for𝜏_{1} exhibit a clear trend, i.e., they decrease with decreasing NPl thickness. Similar
observations have been made in other two-dimensional structures as well, e.g., in GaAs/AlGaAs
quantum wells, for which the relation𝜏_{1}∝ 𝐸_{B}^{−1}was derived.^{78}The thickness dependence of𝐸_{B}for
CsPbBr_{3}NPls has been studied inFigure 4.2 c. In keeping with that, it makes sense that𝜏_{1}decreases
for thinner NPls. Recently, a similar observation was made for MAPbI_{3}NPls.^{12}Another effect that
could lead to faster decay, is that a larger surface-to-volume ratio likely increases the possibility for an
electron to encounter a surface trap, consequently leading to additional nonradiative decay channels.

Compared to the study on GaAs/AlGaAs quantum wells, the lifetimes𝜏_{1}reported here for CsPbBr_{3}
NPls are about one order of magnitude larger.^{78} However, compared to MAPbI_{3} NPls, they are a
factor of two smaller.^{12}Overall, the values given inTable 4.2are already reasonably long lifetimes𝜏_{1}.
However, as previously indicated, in the time-resolved PL data ofFigure 4.9, surface trap repair of
NPls leads to even longer lifetimes, since nonradiative recombination is suppressed by this new PL
enhancement procedure.^{20}This may in turn, also be beneficial for LHP applications relying on exciton
diffusion as longer lifetimes have a direct impact on the exciton diffusion length (seeEquation 2.60).

### Dephasing 5

In recent years, LHPs have experienced a boom in research activity. However, some of their fundamental
properties remain largely unexplored. For example, studies so far rarely distinguish between homogeneous
and inhomogeneous transition broadening. This may be of particular interest for NCs, as inhomogeneous
broadening may also serve as an indicator for the homogeneity of an ensemble of NCs. In this chapter, first,
the total transition broadening will be studied as a function of the sample temperature for three different
LHP NC ensembles: CsPbBr_{3}nanocubes, CsPbBr_{3}nanowires, and MAPbI_{3}nanoplatelets. Based thereon,
the fastest relaxation regime, i.e., the coherent regime, will be examined via four-wave mixing spectroscopy,
yielding the time scale for exciton dephasing in MAPbI_{3}nanoplatelets. These results build a bridge between
the ultrafast polarization decay of exciton ensembles and the respective homogeneous broadening of the
exciton transition. Moreover, it will be shown that exciton wave packets may be generated within these
NCs, leading to quantum beating in the polarization decay signal which can be explained with help of a
three-level system.

97

98 5.1 Total Broadening of Exciton Transitions